ASCE-Jl. of Materials in Civil Engineering, Vol.13,260-273 (2001)
UNIFYING ASPHALT RHEOLOGICAL DATA
USING THE MATERIAL’S VOLUMETRIC-FLOW RATE
Senior Research Fellow
Turner-Fairbank Highway Research Center
6300 Georgetown Pike
McLean, VA 22101
Tel: (202) 493 3105
Fax: (202) 493 3161
The material’s volumetric-flow rate MVR (in cc / 10 minutes) through a predefined die under conditions of constant
temperature and stress has been used for obtaining unified curves of fundamental rheological properties such as
|G*|, G@ and |G*| / Sin * versus frequency in the case of six unmodified asphalts. It has been shown that there is a
theoretical basis for the unification and that the unified curves have far-reaching implications. Since MVR is so
simple to determine quite accurately on a relatively inexpensive, easy-to-use flow measurement device (FMD), this
parameter can be generated on paving sites or at refineries, rather than in research laboratories as is the case with
fundamental rheological parameters. The MVR can then be used as an excellent indicator of the fundamental
rheological parameters through the use of the unified curves.
Keywords : asphalt rheology, unified curves, viscoelastic parameters, flow measurement device, material’s
Asphalts have been recognized as complex materials in terms of their constitution and their rheological behavior. It
is generally accepted that asphalts form a colloidal system represented by a suspension of asphaltene micelles in a
hydrocarbon solvent consisting of saturated paraffins, cycloparaffins and aromatic structures, whose functionality
could vary from polar to non-polar and aliphatic to aromatic. Alternatively, asphalts are viewed as systems in which
amphoteric chemical species, i.e. those containing strong acid and strong base components on the same compound,
are dispersed in a non-polar matrix. In either case, it is this ability to form a colloidal system that lends asphalts
their viscoelastic behavior. The interactions between the colloids lead to the formation of a temporary elastic
network with reversible or partially reversible deformation depending on the deformation time.
Asphalts find major use as binders in road paving applications as well as waterproof coatings in the roofing industry.
The present focus is on paving asphalts though the concepts discussed in the subsequent paragraphs could easily be
applied to the rheology of asphalts in roofing or other fields. Understanding the rheology of paving asphalts is
important from different viewpoints. Primarily, it is useful as a control tool to distinguish between various asphalts
from different crude sources and which are refined using different processes. Secondly, understanding the rheology
of the asphalt helps to properly mix the asphalt with the mineral aggregate at the appropriate temperature and to
compact the composite material in place so that the final pavement can be prepared well and with ease. Thirdly,
understanding asphalt rheology helps to determine how their rheological properties relate to the distresses in the
pavements after the lay down process and after years of service. There is no denying that performance related
criteria are most important because if a distress is prevented or at least alleviated, then economic savings are
gigantic. Asphalts on paved roads are subjected to a wide range of static and dynamic stresses at varying
temperatures and under different environmental conditions. It is essential to develop a good insight into the
rheological properties of the asphalts covering a wide range of shear rates over an equally broad range of
temperatures and under simulated environmental conditions.
With enough important reasons to understand the rheology of asphalts, it is not surprising that there has been a lot of
attention given to this subject over the years. Some of the works include (a) those that sought to study and
recommend various important rheological parameters for asphalts (Anderson et al. 1994; Bahia and Anderson 1995;
Hanson et al. 1995; Dongre et al. 1996), (b) those that modified the asphalts by air blowing, adding various
chemicals or polymers and then studying the rheological properties (Nadkarni et al. 1985; Goodrich 1988;
Shashidhar et al. 1995), ( c ) those that looked for proper equipment to perform fundamental rheological
measurements (Wood and Miller 1960; Schweyer et al. 1976), (d) those that attempted to find methods for rapid
rheological measurements (Griffin et al. 1957; Heukelom 1973; Stroup-Gardiner and Newcomb 1995), (e) those that
searched for relationships between empirical tests and fundamental tests (Van der Poel 1954), (f) those that
identified key rheological parameters as specifications to address major distresses in asphalt pavements (Anderson et
al. 1994) under the Strategic Highway Research Program (SHRP) and so on. The rapid rheological measurements
normally give information on the consistency of the asphalts but do not provide all the fundamental rheological
knowledge about the material. Based on the findings of SHRP (a five-year $150 million dollar United States
research effort established and funded under the 1987 Surface Transportation and Uniform Relocation Assistance
Act), it was concluded that fundamental viscoelastic behavior of asphalts under different levels of stresses and
temperatures needs to be understood for performance-related specifications to address major pavement distresses.
The equipment that provide the fundamental rheological information have a constraint in that they cannot easily be
taken to the field or on-site, normally require highly trained operators and are also relatively much more expensive.
An improved situation will be if one is able to identify a very simple, yet reasonably accurate rheological parameter
that could be determined rapidly on equally simple, low cost instrument and then relate it to fundamental rheological
data in such a way that viscoelastic parameters could be determined through mere calculation rather than actual
experimentation. The present work attempts to bring this idealistic viewpoint to reality and shows a step-by-step
procedure to attain this goal.
SIMPLE RHEOLOGICAL PARAMETER
The simple parameter chosen to give a good measure of the rheological characteristics of asphalt is the material’s
volumetric-flow rate (MVR) that is determined through a closely defined flow measurement device (FMD), whose
main parts are shown in Figure 1.
Figure 1 : Schematic diagram showing the main parts of the Flow Measurement Device (FMD) that is used for
determining the Material’s Volumetric -Flow Rate (MVR).
This equipment is borrowed from the polymer industry where it is routinely used to measure the melt flow index of
the polymers. The cylinder of the flow measurement device is made of hardened steel and is fitted with heaters,
insulated, and controlled for operation at the required temperature. The thermocouple is buried inside the
instrument’s barrel. The thermocouple and the associated temperature control electronics are calibrated against
NIST traceable temperature probes by the equipment manufacturer. The heating device is capable of maintaining
the temperature at 10 mm above the die to within "0.2°C of the desired temperature during the test. The
temperature of the barrel, from 10 mm to 75 mm above the top of the die, is maintained within "1% of the set
temperature ( °C). All this is followed in strict compliance with the ASTM D1238 stipulations. The piston is made of
steel and the diameter of its head is 0.075"0.015 mm less than that of the internal diameter of the cylinder which is
9.5 mm. Extrusion of the material is done through a die made of hardened steel with an internal diameter of 2.095 "
A cursory look at the proposed method to measure the flow parameter may prompt some asphalt rheologists to recall
earlier efforts (Schweyer and Buscot 1971; Schweyer et al. 1976) when a capillary rheometer was used for
generating viscosity data. Initially (Schweyer and Buscot 1971), experiments were conducted at a constant rate of
strain but later (Schweyer et al. 1976) a constant stress mode was employed for mo re rapid testing. The approach
did not become popular because of the large shear stresses and strains that were produced during measurement.
These could lead to spurious results under certain conditions of high stresses due to the elasticity of the material and